Download presentation

Presentation is loading. Please wait.

Published byShreya Baston Modified over 4 years ago

1
**Structural Engineering Lecture Series – September 22, 2007**

Advanced Composite Material Applications in Structural Engineering Advances and Challenges By Amjad J. Aref Associate Professor Structural Engineering Lecture Series – September 22, 2007

2
**OUTLINE Introduction: What are Composite Materials?**

Bridge Applications Final Remarks

3
**What are Composite Materials?**

Composite structures are often called fiber reinforced polymer (FRP) structures, and polymer matrix composites (PMC). Composite materials are man-made, and must contain at least two constituents that are distinct chemically and physically. Intended to achieve an increase in certain properties such as stiffness, strength, fracture toughness among others, or decrease certain properties such as weight and corrosion. Composites in general can be categorized in two groups as follows:

4
**Composites Architecture**

Reinforcement Interface Matrix

5
Reinforcement Long continuous bundles l/d > 10 by definition, (typical dia for a fiber ~ 6-15 µm) unidirectional multidirectional woven or braided Continuous fibers Short chopped fibers randomly oriented Whiskers long thin crystals d< 1 micron length in the order of 100 microns used in ceramic matrix composites (CMC) and metal matrix composites (MMC) Particulates Near spherical not usually used for strength increase the toughness of the material Flakes metallic, electrical/heating applications 2-D in nature, not usually used for strength

6
**Reinforcement (cont’d)**

Glass (E-, S-, C-glass fibers) E-glass: Young’s modulus ~ 72 GPa, σu=3450 MPa (500 ksi ), Strain to failure 1-2% Carbon EL: GPa, ET=12-20 GPa σu= MPa ( ksi), strain to failure 0.5-1% Kevlar, Spectra (organic) E: GPa σu= MPa ( ksi), strain to failure 2-5% Ceramic fibers: high strength, stiffness and temperature stability Alumina (Al2O3) E: 370 GPa σu=1380 MPa (200 ksi) SiC Boron (toxic material), typically large diameter

7
Matrix Metallic Ceramic Polymeric Thermoplastic Thermoset

8
Polymer Matrix Poly mer Linear Branched Cross-linked Network

9
**Composites Categories**

Reinforced Plastics Low strength and stiffness Inexpensive Glass fibers is primary reinforcement Applications: Boat Hulls Corrugated sheets Piping Automotive panels Sporting goods Advanced Composites High strength and stiffness Expensive High performance reinforcement such as: graphite, aramid, kevlar Applications: Aerospace industry

10
**Typical Applications in Structural Engineering**

Retrofitting of beams and columns Seismic Retrofitting New applications Bridge Deck Bridge Superstructure

11
**FRP COMPOSITES IN STRUCTURAL APPLICATIONS**

Advantages High specific strength and stiffness Corrosion resistance Tailored properties Enhanced fatigue life Lightweight Ease of installation Lower life-cycle costs Factors preventing FRP from being widely accepted High initial costs No specifications No widely accepted structural components and systems Insufficient data on long-term environmental durability

12
**CONDITIONS OF U.S. HIGHWAY BRIDGES**

28% of 590,000 public bridges are classified as “deficient”. The annual cost to improve bridge conditions is estimated to be $10.6 billion. Need for bridge systems that have long-term durability and require less maintenance (Source: National Bridge Inventory)

13
**Demand for FRP in Bridge Applications**

Is it necessary to use expensive FRP materials for bridge renewal? Given the massive investment to renew deficient bridges (28% of all bridges are deficient), repeating the same designs, materials, etc. may not be a prudent approach. Consider the fact that the average life span of a bridge in the U.S. is 42 years. FRP materials, if designed properly, could provide new bridges that last over 100 years.

14
**GLASS FIBER REINFORCED POLYMER (GFRP) BOX SECTIONS**

The compressive flange is weaker than the tensile flange. A failure of a GFRP box section usually occurs in a catastrophic manner. The design of a GFRP box section is usually governed by stiffness instead of strength. Hybrid design or Special structural system

15
**BRIDGE APPLICATIONS – 1 (TOM’S CREEK BRIDGE)**

203 mm 152 mm Virginia Tech and Strongwell Pultruded composite beam (hybrid design of glass and carbon fibers and vinyl ester matrix) Span : 5.33 m , Width : 7.32 m

16
**BRIDGE APPLICATIONS – 2 (TECH 21 BRIDGE)**

LJB Engineers & Architects, Inc. and Martin Marietta Materials Length : 10.1 m, Width : 7.3 m E-glass fiber reinforcement and polyester matrix Deck : pultruded trapezoidal tubes between two face sheets (tubes run parallel with the traffic direction) Stringer : three U-shaped structural beams 838 mm

17
**BRIDGE APPLICATIONS – 3 (KINGS STORMWATER CHANNEL BRIDGE)**

UC San Diego, Alliant TechSystems, Inc., and Martin Marietta Span: 2 x 10 m, Width: 13 m Six longitudinal concrete filled carbon tube girders (carbon/epoxy system) GFRP deck panel (pultruded trapezoidal E-glass/epoxy tubes with a top skin layer GFRP deck Filament wound CFRP tube

18
**BRIDGE APPLICATIONS – 4 (TOOWOOMBA BRIDGE)**

University of Southern Queensland, Wagners Composite Fibre Technologies, and Huntsman Composites Span : 10 m, Width : 5.0 m Hybrid box beams : prefabricated concrete, GFRP, and CFRP 350 450 100 (dimensions in mm) concrete GFRP CFRP

19
**MARKET SHARE (FRP COMPOSITES)**

20
**FRP COMPOSITE SHIPMENTS**

21
**Recent Development of FRP Bridge Deck and Superstructure Systems**

22
**Hybrid-FRP-Concrete Bridge Deck and Superstructure System**

The system is developed at UB by an optimum selection of concrete and FRP. The system is validated analytically and experimentally to assess the feasibility of the proposed hybrid bridge superstructure and deck. Simple methods of analysis for the proposed hybrid bridge superstructure were developed.

23
**BASIC CONCEPT OF PROPOSED HYBRID FRP-CONCRETE BRIDGE**

Single span with a span length of 18.3 m AASHTO LRFD Bridge Specifications Live load deflection check dLL<L/800 under (1+IM)Truck Service I limit DC+DW+Lane+(1+IM)Truck Strength I limit 1.25DC+1.5DW+1.75[Lane+(1+IM)Truck] Concrete should fail first in flexure. A strength reduction factor for GFRP was taken as 0.4. 18288 mm 99mm 1160 mm 3785 mm Simple-span one-lane hybrid bridge

24
**PROPOSED HYBRID BRIDGE SUPERSTRUCTURE**

Advantages include: Increase in stiffness Corrosion resistance Cost-effectiveness Lightweight Local deformation reduction High torsional rigidity Pre-fabrication Short construction period

25
**DISPLACEMENT AND STRENGTH CHECKS**

Deflection check: 0.61 x L/800 Max. failure index : (safety factor=3.1) (a) Live load deflection check (b) Tsai-Hill Failure index under Strength I limit

26
**TSAI-HILL FAILURE INDEX**

Failure condition : where Strengths in the principal 1 and 2 directions and in-plane shear Tensile and compressive directions

27
**EXPERIMENTAL PROGRAM Materials Non-destructive tests Fatigue test**

GFRP Concrete Non-destructive tests Flexure Off-axis flexure Fatigue test Destructive tests Shear Bearing

28
**TEST SPECIMEN One-fifth scale model Span length = 3658 mm**

(dimensions in mm)

29
STACKING SEQUENCES Thickness of one layer = mm

30
FABRICATION – 1

31
FABRICATION – 2

32
SHEAR KEYS Shear keys (dimensions in mm) Longitudinal direction

33
**MATERIALS – GFRP Cheaper than carbon fiber reinforcement**

Fill Warp E-glass woven fabric reinforcement Cheaper than carbon fiber reinforcement Impact resistance Vinyl ester High durability Extremely high corrosion resistance Thermal stability Material Properties Test Dir. E or G (GPa) n Strength (MPa) Tens Fill 16.6 0.129 285 Warp 17.9 0.131 335 Comp 15.9 0.099 -241 22.5 0.254 -265 Shear 2.72 -- 56.1 2.45 63.8

34
GFRP – TENSION

35
GFRP – COMPRESSION

36
GFRP – SHEAR

37
**MATERIALS - CONCRETE No coarse aggregates**

water : cement : aggregate = 0.46 : 1.0 : 3.4 by weight Compressive Properties Young’s Modulus (GPa) Strength (MPa) 8.38 37.9

38
TEST SETUP

39
**FLEXURAL LOADING CONFIGURATION**

(dimensions in mm) (a) Elevation (b) Cross section (flexure) (c) Cross section (off-axis flexure)

40
**NONDESTRUCTIVE FLEXURE (TEST PROTOCOL)**

To examine elastic behavior of the bridge under the flexural loading Displacement control Max applied displ = L/ (L: span length)

41
**NONDESTRUCTIVE FLEXURE (FORCE-DISPLACEMENT)**

19% increase 40% for the prototype

42
**NONDESTRUCTIVE FLEXURE (TOP SURFACE DEFORMATION)**

43
**NONDESTRUCTIVE FLEXURE (STRAIN RESULTS)**

Bottom surface along the center-line (b) Exterior web over height

44
**FATIGUE LOADING (TEST PROTOCOL)**

To examine fatigue characteristics Flexural loading Force control 2 x 106 cycles Freq.= 3.0 Hz Max. load = 2.0 x Tandem Stiffness evaluation every 0.2 million cycles

45
**FATIGUE LOADING (TEST RESULTS)**

46
**DESTRUCTIVE FLEXURE (TEST PROTOCOL)**

To examine the strength of the bridge and failure modes Flexural loading Displacement control Two stages Step I (displacement history #1) Step II (displacement history #2) (a) Displacement history #1 (b) Displacement history #2

47
**DESTRUCTIVE FLEXURE (TEST RESULTS – 1)**

Failure load = 35 x Tandem load local global

48
**CHANGE OF A LOADING CONDITION**

From four point loads to two line loads contact

49
**DESTRUCTIVE FLEXURE (TEST RESULTS – 2)**

Failure modes Concrete crushing Failure of GFRP in compression

50
**DESTRUCTIVE FLEXURE (FAILURE MODES)**

51
SHEAR TEST

52
BEARING TEST

53
**BEARING TEST (FAILURE MODE)**

54
**FINITE ELEMENT ANALYSIS**

ABAQUS Four-noded general shell element, S4R, for GFRP laminates Eight-noded general 3D solid element, C3D8, for concrete Assumed a perfect bonding between concrete and GFRP Linear analysis Nonlinear analysis

55
**FINITE ELEMENT DISCRITIZATION (LINEAR ANALYSIS)**

Number of nodes: 31,857 Number of elements: 38,892 (22,764 for S4R and 16,128 for C3D8)

56
**LINEAR FEA RESULTS (FLEXURE – 1)**

Stiffness was predicted by FEA within 5% error.

57
**LINEAR FEA RESULTS (FLEXURE – 2)**

(a) Top surface (b) Bottom surface

58
**LINEAR FEA RESULTS (FLEXURE – 3)**

Bottom surface along the center-line (b) Exterior web over height

59
**FINITE ELEMENT DISCRETIZATION (NONLINEAR ANALYSIS)**

A quarter model x y Loading point

60
**NONLINEAR FEA RESULTS – 1**

61
**NONLINEAR FEA RESULTS – 2 (DAMAGED AREA)**

x y failure section (a) FEA (b) Experiment

62
**SIMPLE METHODS OF ANALYSIS**

Beam analysis Orthotropic plate analysis Classical lamination theory Use of effective engineering properties of laminates Perfect bonding between concrete and GFRP was assumed. Shear deformation was neglected Primary objective is to obtain deflection under design loads.

63
BEAM ANALYSIS The bridge is modeled as a beam with a span length, L, effective flexural rigidity, EIeff, and effective torsional rigidity, GJeff. where Effective modulus Effective shear modulus Vertical coord. from the neutral axis Area enclosed by median lines of the top and bot. flanges and exterior webs Axis along the median line of a component

64
**ORTHOTROPIC PLATE ANALYSIS**

The bridge is modeled as an orthotropic plate with span length of L and width of W. where Vertical displacement Distributed load on the plate Rigidities that can be obtained by using the classical lamination theory

65
**REPRESENTATIVE UNITS FOR THE PLATE ANALYSIS**

(a) Longitudinal direction (b) Transverse direction

66
**SIMPLE METHODS OF ANALYSIS (UNDER TANDEM LOAD ONLY)**

(a) Transverse direction (b) Longitudinal direction

67
Summary Composite materials hold great promise for effective renewal of deficient bridges. The hybrid FRP-concrete bridge superstructure is highly feasible from the structural engineering point of view. GFRP used in this study has revealed that its stress-strain relationship is not perfectly linear-elastic. However, for design purposes, the equivalent linear model can be used.

68
Summary (CONT’D) As is often the case with all-composite bridges, the design of the hybrid bridge superstructure is also stiffness driven. Results from a series of quasi-static tests have shown an excellent performance of the proposed hybrid bridge under live loads. The beam and orthotropic plate simplified analyses have proven to be effective to accurately predict the deflection of the hybrid bridge under design loads.

69
Challenges A systematic way to determine design parameters should be developed. It is also important to propose and optimize the design based on life-cycle cost as well as performance. Long-term performance of FRP bridges is not yet established and should be investigated: creep, fatigue, and material degradation. Thermal effects on FRP bridges is still unknown and should be investigated. Quality control concerns— the material properties are highly dependent on the manufacturing process.

70
Challenges (CONT’D) Several practical aspects of FRP applications in bridges need to be addressed by researchers. The following are some of the outstanding issues: Methods to expand lanes Methods to cast concrete Considerations for negative moments Concrete barrier or steel parapet Support conditions

71
Challenges (CONT’D) There are benefits in using light FRP deck or superstructure in bridges located in moderate and seismic regions. Automated fabrication process must be used to fabricate the FRP parts of the superstructure or deck.

72
**AUTOMATED FABRICATION PROCESSES**

Pultrusion RTM VARTM Use of braided fabrics Filament Winding

73
**Acknowledgment Dr. Y. Kitane Dr. W. Alnahhal**

New York State Department of Transportation

74
THANK YOU

Similar presentations

Presentation is loading. Please wait....

OK

Chap.8 Mechanical Behavior of Composite

Chap.8 Mechanical Behavior of Composite

© 2018 SlidePlayer.com Inc.

All rights reserved.

To make this website work, we log user data and share it with processors. To use this website, you must agree to our Privacy Policy, including cookie policy.

Ads by Google